Click here to load reader

View

0Download

0

Embed Size (px)

UntitledSubmitted on 28 Feb 2019

HAL is a multi-disciplinary open access archive for the deposit and dissemination of sci- entific research documents, whether they are pub- lished or not. The documents may come from teaching and research institutions in France or abroad, or from public or private research centers.

L’archive ouverte pluridisciplinaire HAL, est destinée au dépôt et à la diffusion de documents scientifiques de niveau recherche, publiés ou non, émanant des établissements d’enseignement et de recherche français ou étrangers, des laboratoires publics ou privés.

Young’s Modulus of Austenite and Martensite Phases in Superelastic NiTi Wires

Petr Šittner, Ludek Heller, Jan Pilch, Caroline Curfs, Thierry Alonso, Denis Favier

To cite this version: Petr Šittner, Ludek Heller, Jan Pilch, Caroline Curfs, Thierry Alonso, et al.. Young’s Modulus of Austenite and Martensite Phases in Superelastic NiTi Wires. Journal of Materials Engineering and Performance, Springer Verlag/ASM International, 2014, 23 (7), pp.2303-2314. 10.1007/s11665-014- 0976-x. hal-02022634

Youngs Modulus of Austenite and Martensite Phases in Superelastic NiTi Wires

Petr Sittner, Ludek Heller, Jan Pilch, Caroline Curfs, Thiery Alonso, and Denis Favier

Youngs moduli of superelastic NiTi wires in austenite and stress-induced martensite states were evaluated by three different experimental methods (tensile tests, in situ synchrotron x-ray diffraction, and dynamic mechanical analysis) and estimated via theoretical calculation from elastic constants. The unusually low value of the Youngs modulus of the martensite phase appearing in material property tables (<40 GPa) is generally ascribed in the literature to the fact that stress-driven martensitic transformation and/or twinning processes continue even beyond the transformation range and effectively decrease the value of the tangent modulus evaluated from macroscopic stress-strain curve. In this work, we claim that this low value is real in the sense that it corresponds to the appropriate combination of elastic constants of the B19¢ martens- ite phase forming the polycrystalline wire. However, the Youngs modulus of the martensite phase is low only for wire loaded in tension, not for compression or other deformation modes. It is shown that the low value of the martensite Youngs modulus in tension is due to the combination of the unique coincidence of elastic anisotropy of the B19¢ martensite characterized by the low elastic constant C55, austenite drawing texture, and strong martensite texture due to the martensite variant selection under tensile stress.

Keywords mechanical, modeling and simulation, non-ferrous metals

1. Introduction

elastic, transformation, and thermal expansion strains. For

general understanding and modeling the SMA functional

responses as well as for the development of SMA devices, it

is essential to mutually separate and evaluate these strains.

Since in superelastic technologies focused at SMST we are

dealing with recoverable strains of polycrystalline NiTi ele-

ments at constant temperature, thermal expansion is neglected

here. However, distinction between elastic and transformation

strains of NiTi polycrystal is already complicated, since it relies

upon the knowledge of the elastic moduli of the austenite and

martensite phases which is not trivial. Material property tables

specify ‘‘elastic properties of NiTi’’ separately for austenite

and martensite using relatively wide ranges, e.g., (Ref 1) as

41-75 GPa for the Youngs modulus of the B2 austenite and

28-41 GPa for that of the B19¢ martensite. Such uncertainty is

hardly acceptable for engineers designing superelastic NiTi

devices, and it is suspicious that Youngs modulus of martensite is

lower than that of the austenite. On top of that, elastic moduli of

both phases vary strongly with temperature (Ref 2), and martensite

moduli may depend on the history; particularly, they can be

different in tension and compression. So, there are some good

reasons for the intervals appearing in material property tables.

In fact, the uncertainty in elastic moduli of NiTi originates

mainly from (i) experimental difficulties associated with

reliable determination of elastic constants, and (ii) temperature

and history dependence of the effective Youngs modulus of the

wire associated with the martensitic transformation. Besides

that, however, there is one more extremely important issue. In

contrast to conventional materials, stress-induced phase trans-

formations and/or twinning processes in SMAs create internal

interfaces which are highly responsive to external stress. These

interfaces may exist in the microstructure even at temperatures

and macroscopic stresses far from the equilibrium transforma-

tion condition (far from the equilibrium transformation line in

stress-temperature space). These mobile interfaces make it

difficult to evaluate elastic properties of NiTi by conventional

means from macroscopic stress-strain curves.

Elastic constants of austenite and martensite phases in

SMAs can be beneficially measured on single crystals without

applying external macroscopic stress by ultrasonic methods,

particularly by resonant ultrasound spectroscopy (Ref 3, 4).

However, since it is difficult to prepare NiTi martensite single

crystal in a quality sufficient for the acoustic measurement,

there are no reliable experimental data for elastic constants of

the B19¢ martensite in the literature yet.

Given the lack of knowledge of elastic constants of the B19¢

martensite, theoreticians recently attempted to calculate them

from the first principles (Ref 5-7). All the available results seem

to suggest that martensite shall be the elastically harder phase,

which clearly contradicts the overwhelming experimental

evidence from tensile tests in the literature showing that

Youngs modulus of superelastic NiTi wire stretched beyond

This article is an invited paper selected from presentations at the International Conference on Shape Memory and Superelastic Technologies 2013, held May 20-24, 2013, in Prague, Czech Republic, and has been expanded from the original presentation.

Petr Sittner, Ludek Heller, and Jan Pilch, Institute of Physics, ASCR, Prague, Czech Republic. Caroline Curfs, ESRF, Grenoble, France; and Thiery Alonso and Denis Favier, Universite de Grenoble, Grenoble, France. Contact e-mail: [email protected]

1

the transformation plateau into stress-induced martensite

(Fig. 1a) is lower than in the austenite phase prior the plateau.

The low martensite modulus of NiTi has been a longstanding

puzzle in the SMA field. Hence, we decided to look at it more

closely in this work.

Wayne Metals, NiTi #1, straight annealed, d = 0.1 mm, was

used in present experiments. Youngs moduli of the austenite

and stress-induced martensite in these wires were evaluated by

three experimental methods (tensile tests, in situ synchrotron

x-ray diffraction, and dynamic mechanical analysis). Figure 1a

shows superelastic stress-strain curve of this wire stretched in

tension till fracture, yielding values of the static Youngs moduli

EA = 66.8 GPa (austenite) and EM = 24.8 GPa (martensite).

Electrical resistivity of the wire measured during the tensile test

is superimposed. Note that the electrical resistivity increases

with increasing stress both prior and after the plateau. It should

stay constant, if there was elastic deformation only. It is known

(Ref 8, 9) that, prior the plateau, this is due to the deformation

processes related with R-phase and due to twinning and

transformation after the plateau. So, it is obvious that evaluation

of the Youngs moduli from macroscopic responses in tensile

tests on NiTi wires is thus highly questionable.

An alternative way which can be used for evaluating the

elastic responses of solids regardless of the activity of other

deformation processes in the studied sample is the in situ x-ray

(neutron) diffraction method (Ref 10). In these methods, lattice

strain ehkl is evaluated (Eq. 1) from the relative changes of the

lattice spacing dhkl (position of the hkl diffraction peak in the

diffraction pattern) with increasing applied stress r. d0,hkl is the

lattice spacing in stress-free state.

ehkl ¼ dhkl d0;hklÞ=d0;hkl

ðEq 1Þ

To evaluate the strain component along thewire (load) axis, the

diffracting lattice planes must be oriented perpendicularly to the

load axis. Obviously, the strains ehkl evaluated from the changes of

lattice spacings (shift of diffraction peaks) are elastic strains only.

Since the intensity of the diffraction peak originates from a set of

equally oriented grains of a particular phase within the gage

volume of the polycrystalline wire, the lattice strains are oriented

and phase-sensitive values that are averaged over the gage volume.

If the values of lattice strains for various reflections are plot against

the applied stress r, the slopes of these dependences (Eq. 2) yield

so-called diffraction elastic moduli,Dhkl, characterizing the elastic

properties of thematerial. If thematerial is not toomuch elastically

anisotropic, then the slopes Dhkl for individual reflections are

similar each other and their average value approaches the Youngs

modulus of the polycrystal.

Dhkl ¼ r=ehkl ðEq 2Þ The in situ synchrotron x-ray experiments in this work were

performed using miniature deformation rig (Ref 11) installed on

high-resolution powder diffractometer ID31 at ESRF Grenoble.

The results for austenite and stress-induced martensite existing in

the thin NiTi wire under applied tensile stress are given in Fig. 2

and 1, respectively. The average value of austenite diffraction

moduli DA = 70 GPa is not that far from the value of Youngs

modulusmeasured in the stress-strain test. The stress-strain curves

in Fig. 2a and 1a are different, since theNiTi wirewas additionally

annealed (Fig. 2a) to avoid the R-phase (18 ms/125 W treatment

in Ref 11) complicating the analysis of the diffraction measure-

ments prior the stress plateau. Applying the same method to the

evaluation of elastic response of martensite is, however, a bit more

complicated, since it is not straightforward to measure the stress-

free lattice spacings d0,hkl (martensite does not exist without stress

at room temperature). On the other hand, we can measure more

lattice strain-stress dependences (Fig. 3), since there is more

martensite peaks in the martensite diffraction patterns (Fig. 1b).

d0,hkl for each martensite reflection was found by extrapolating the

linear lattice strain-stress dependences to zero stress. The results

clearly show that the orientation-dependent diffraction elastic

moduliDhkl of themartensite are systematically higher (DM 120

GPa), and the martensite phase is more elastically anisotropic than

the austenite. The results thus contradict the low value of the

martensite modulus evaluated from the tensile test.

Third method used to evaluate elastic properties of the NiTi

wire was dynamic mechanical analysis. Theoretically, the

dynamic modulus E¢ evaluated by this method from small

amplitude vibrations superimposed over the macroscopic static

stress-strain should not be affected by the activity of other

deformation mechanism acting in the wire. Although this is the

case for plasticity, it is not true for deformation processes derived

from the martensitic transformation which are accompanied by

Fig. 1 a) Tensile r-e curve of superelastic NiTi wire (FWM #1,

d = 0.1 mm) at room temperature. Electrical resistivity of the wire

measured during the tensile test is superimposed. (b) In situ x-ray

diffraction patterns evaluated under applied tensile stress (denoted by

points on r-e curve in (a) in axial geometry (diffracting planes per-

pendicular to wire axis)

2

the phase change or lattice orientation changes giving rise to the

mobile internal interfaces. Figure 4 shows the evolution of E¢

during a superelastic test on NiTi wire at room temperature till

fracture (Fig. 4a) and during cyclic superelastic test at T = 37 C

(Fig. 4b). Note that, prior the start of martensitic transformation,

the dynamic elastic modulus E¢ increases with stress at lower

temperature T = 19 C, while at higher temperature T = 37 C, it

decreases. This is the effect of the R-phase. The change of the E¢

with the applied stress during stress-induced B2-R transformation

has a form of U-shape. We see only the second branch of the U at

lower temperature T = 19 C (Fig. 4a), while only the first branch

of it at T = 37 C (Fig. 4b). If there is no R-phase, E¢ stays

constant during the elastic loading of the austenite (Fig. 2a). This

method can be used in principle to evaluate the elastic properties

(E¢) of the NiTi wire also in case of phase mixtures (1-7% strain)

within the transformation range, see the hysteretic variation ofE¢ in

Fig. 4b. The variation of E¢ with strain is not U-shaped but linear

due to thepropagationof localizeddeformation in shear bands.The

most important information to be inferred from Fig. 4, however, is

that, although the dynamic elastic modulus E¢ of martensite

increases with increasing stress beyond the plateau, it never

exceeds a maximum value of E¢ 50 GPa (Fig. 4a). The E¢

increases upon stressing the wire beyond the transformation

plateau since the twinning and transformation processes continue

beyond the plateau but their activity gradually expires. The

maximum of the E¢ 50 GPa observed at 10% strain corresponds

to their complete expiration not due to the onset of the plasticity.

3. Theoretical Calculations

mental results presented above, we tried to estimate Youngs

moduli of the B2 austenite phase and stress-induced monoclinic

B19¢ martensite phase in NiTi wire by theoretical calculations.

The idea is rather simple. First, we calculated single crystal

Fig. 2 Elasticity of the austenite evaluated from x-ray diffraction experiment on the high-resolution diffractometer ID31 at ESRF Grenoble, (a) tensile

r-e curve of the same NiTi wire additionally heat treated to avoid R-phase, Electrical resistivity of the wire measured during the tensile test is superim-

posed, (b, c) peak shifts measured in the diffraction experiment at tensile stresses denoted on the r-e curve in (a). Broad yellow profiles were obtained

after unloading after full superelastic cycle, (d) lattice strain-stress diagram showing linear ‘‘lattice plane responses’’ of various austenite hkl reflections

(Color figure online)

Fig. 3 Elasticity of martensite evaluated from the x-ray diffraction

experiment on the high-resolution diffractometer ID31 at ESRF Gre-

noble. Diffraction elastic moduli Dhkl of austenite and martensite

appearing as slopes of the lattice strain-stress dependence (measure-

ment points in Fig. 1a beyond the plateu)

3

Youngs modulus Ehkl along a given austenite crystal direction

hklA, and check how it changeswith the stress-inducedmartensitic

transformation in tension/compression. Ideally, this would corre-

spond to the slope of elastic response of austenite single crystal

loaded in tension/compression along the hkl direction prior and

after the stress-induced transformation. The single-crystal moduli

were calculated based on the knowledge of (i) crystal lattice

parameters and (ii) elastic constants of both austenite and

martensite phases, (iii) lattice correspondence between austenite

and martensite yielding information on how particular austenite

crystal direction transforms into the product phase, and (iv)

martensite variant selection rule telling which martensite variant

will form by the application of uniaxial tensile and compressive

strain along particular austenite crystal direction. Figures 7 and 8

inform the orientation and sense of loading dependence of the

single-crystal moduli. Finally, the polycrystalline Youngs moduli

are estimated taking into account grain constraints and textures.

3.1 Input Parameters

B19¢ martensite phases are listed in Table 1 including matrices

used for transforming Miller indexes hkl into vectors in

Cartesian system (xyz) aligned with lattice unit cells of

austenite and martensite. Matrix operators, lattice correspon-

dence, and related matrix operators are given in Table 2, and

finally, elastic constants of the austenite and martensite phases

taken from literature (Ref 5, 12, 13) are given in Table 3.

3.2 Martensite Variant Selection Rule

In order to evaluate how Youngs modulus of the austenite

single crystal will change with stress-induced martensitic

transformation when loaded along a specific direction in

tension/compression, one has to decide which one of the 12

martensite variants will form, i.e., one needs to adopt a

martensite variant selection rule. This is already an approxi-

mation, since we implicitly assume here that the austenite

single crystal will transform into a single martensite variant,

which yields maximum transformation strain into the load axis

direction and sense of loading (tension or compression).

In order to apply the above martensite variant selection rule,

we calculated orientation dependence of transformation strains

for all 12 martensite variants using transformation matrix

T xyz B2!B190 relating crystal directions of B2 austenite (uvw)T and

B19¢ martensite (UVW)T in the Cartesian system aligned with

B2 austenite unit cell (Eq. 3). In these calculations, lattice

parameters with related operators (Table 1) and austenite/

martensite lattice correspondence with related operators

(Table 2) are used.

u

v

w

0

hkl!xyz TB2 hkl!xyz Thkl

matrix Ui that is computed through polar decomposition of the

transformation matrix T xyz B2!B190 defined for each variant. Then,

engineering strain was used to calculate transformation strain

tensor ei i.e., ei = 1/2(Ui T + Ui) I, where I stands for 39 3

identity matrix. Orientation dependence of tensile/compressive

transformation strains was evaluated through projection of the

transformation strain tensor to all orientations i.e., tensile/

compressive transformation strain for variant i along direction

e = eTei e. The results for martensite variant 3 are shown in

Fig. 5. Orientation dependence of the maximum transformation

strain in compression (a) and tension (b) in a single quadrant of

austenite coordinate system are shown in Fig. 6. Note that (i)

transformations strains are statistically larger in tension than in

compression, and (ii) while one martensite variant is sufficient

to be considered within the basic stereographic triangle in

tension, three martensitic variants need to be considered in

compression.

From the above calculation, we know the load axis orienta-

tions within the martensite phase which corresponds to each

austenite crystal direction and sense of loading. Based on this, we

calculate orientation dependence of the single crystal Youngs

moduli using the elastic constants and show it in Table 3

(constants from Ref 5 were used). The results for martensite

variant 3 yielding largest strains in tension are shown in Fig. 7,

and for three martensite variants 1, 5, and 9 yielding larger

transformation strains in compression in are shown in Fig. 8.

Since plot of four surfaces in a single figure are difficult to inspect,

sections along {011} austenitic planes are shown.

Fig. 4 Tensile r-e curves of superelastic NiTi wire (NiTi #1, d = 0,

1 mm) with superimposed dynamic modulus E’ evaluated in DMA

experiment using frequency f = 30 Hz (a) at room temperature T = 19 C

till fracture and (b) cyclic test at ambient temperature T = 37 C

4

3.4 Effect of Grain Interactions and Texture on Polycrystalline Youngs Moduli

The next step should be to calculate Youngs modulus of

polycrystalline wire. Since the wire is not a set of isolated

crystals but a polycrystalline aggregate, in which the individual

single crystal grains mutually interact when exposed to external

loading, an averaging homogenization scheme must be adopted

to calculate homogenized polycrystalline Youngs modulus

(Ref 14-16). Although this topic has been widely addressed in

the literature, there are issues making it difficult to be applied to

NiTi wires as follows: (i) the crystal orientations are not

distributed randomly in the aggregate but some grain orienta-

tions prevail due to the strong texture of the thin wire (Fig. 9),

(ii) it is not realistic that whole grain transforms into one of the

12 lattice correspondent variants in Table 2, and (iii) it is not

realistic that the wire transforms fully to the martensite state

under stress. Typical NiTi wire texture results in a preferential

orientation of polycrystal grains along the 111A direction as

Fig. 9 shows. Although the latest averaging schemes published

in the literature go much far beyond the Voigt and Reuss

approximations allowing for taking into account the effects of

texture (Ref 16), grain size distribution (Ref 15), and even

multiphase microstructure (Ref 14) of the polycrystal, their

application to NiTi polycrystal in martensite state is still

problematic. There is one major critical issue-if we want to

compare the theoretical and experimental results, we need to

assure that the phase and twin interfaces do not move under the

increasing applied stress. Since we are lacking reliable inputs

for i-iii needed for homogenization and since the aim of this

work was mainly to clarify the long-lasting puzzle of the low

martensitic modulus of NiTi in material property tables,

polycrystalline Youngs moduli were not calculated but only

estimated in this work.

4.1 Youngs Modulus of the Wire in Austenite Phase

The values of the Youngs modulus of the polycrystalline

austenite phase evaluated by all methods converge around

E = 70 GPa. Theoretically calculated value of the

homogenized polycrystal Youngs modulus…

HAL is a multi-disciplinary open access archive for the deposit and dissemination of sci- entific research documents, whether they are pub- lished or not. The documents may come from teaching and research institutions in France or abroad, or from public or private research centers.

L’archive ouverte pluridisciplinaire HAL, est destinée au dépôt et à la diffusion de documents scientifiques de niveau recherche, publiés ou non, émanant des établissements d’enseignement et de recherche français ou étrangers, des laboratoires publics ou privés.

Young’s Modulus of Austenite and Martensite Phases in Superelastic NiTi Wires

Petr Šittner, Ludek Heller, Jan Pilch, Caroline Curfs, Thierry Alonso, Denis Favier

To cite this version: Petr Šittner, Ludek Heller, Jan Pilch, Caroline Curfs, Thierry Alonso, et al.. Young’s Modulus of Austenite and Martensite Phases in Superelastic NiTi Wires. Journal of Materials Engineering and Performance, Springer Verlag/ASM International, 2014, 23 (7), pp.2303-2314. 10.1007/s11665-014- 0976-x. hal-02022634

Youngs Modulus of Austenite and Martensite Phases in Superelastic NiTi Wires

Petr Sittner, Ludek Heller, Jan Pilch, Caroline Curfs, Thiery Alonso, and Denis Favier

Youngs moduli of superelastic NiTi wires in austenite and stress-induced martensite states were evaluated by three different experimental methods (tensile tests, in situ synchrotron x-ray diffraction, and dynamic mechanical analysis) and estimated via theoretical calculation from elastic constants. The unusually low value of the Youngs modulus of the martensite phase appearing in material property tables (<40 GPa) is generally ascribed in the literature to the fact that stress-driven martensitic transformation and/or twinning processes continue even beyond the transformation range and effectively decrease the value of the tangent modulus evaluated from macroscopic stress-strain curve. In this work, we claim that this low value is real in the sense that it corresponds to the appropriate combination of elastic constants of the B19¢ martens- ite phase forming the polycrystalline wire. However, the Youngs modulus of the martensite phase is low only for wire loaded in tension, not for compression or other deformation modes. It is shown that the low value of the martensite Youngs modulus in tension is due to the combination of the unique coincidence of elastic anisotropy of the B19¢ martensite characterized by the low elastic constant C55, austenite drawing texture, and strong martensite texture due to the martensite variant selection under tensile stress.

Keywords mechanical, modeling and simulation, non-ferrous metals

1. Introduction

elastic, transformation, and thermal expansion strains. For

general understanding and modeling the SMA functional

responses as well as for the development of SMA devices, it

is essential to mutually separate and evaluate these strains.

Since in superelastic technologies focused at SMST we are

dealing with recoverable strains of polycrystalline NiTi ele-

ments at constant temperature, thermal expansion is neglected

here. However, distinction between elastic and transformation

strains of NiTi polycrystal is already complicated, since it relies

upon the knowledge of the elastic moduli of the austenite and

martensite phases which is not trivial. Material property tables

specify ‘‘elastic properties of NiTi’’ separately for austenite

and martensite using relatively wide ranges, e.g., (Ref 1) as

41-75 GPa for the Youngs modulus of the B2 austenite and

28-41 GPa for that of the B19¢ martensite. Such uncertainty is

hardly acceptable for engineers designing superelastic NiTi

devices, and it is suspicious that Youngs modulus of martensite is

lower than that of the austenite. On top of that, elastic moduli of

both phases vary strongly with temperature (Ref 2), and martensite

moduli may depend on the history; particularly, they can be

different in tension and compression. So, there are some good

reasons for the intervals appearing in material property tables.

In fact, the uncertainty in elastic moduli of NiTi originates

mainly from (i) experimental difficulties associated with

reliable determination of elastic constants, and (ii) temperature

and history dependence of the effective Youngs modulus of the

wire associated with the martensitic transformation. Besides

that, however, there is one more extremely important issue. In

contrast to conventional materials, stress-induced phase trans-

formations and/or twinning processes in SMAs create internal

interfaces which are highly responsive to external stress. These

interfaces may exist in the microstructure even at temperatures

and macroscopic stresses far from the equilibrium transforma-

tion condition (far from the equilibrium transformation line in

stress-temperature space). These mobile interfaces make it

difficult to evaluate elastic properties of NiTi by conventional

means from macroscopic stress-strain curves.

Elastic constants of austenite and martensite phases in

SMAs can be beneficially measured on single crystals without

applying external macroscopic stress by ultrasonic methods,

particularly by resonant ultrasound spectroscopy (Ref 3, 4).

However, since it is difficult to prepare NiTi martensite single

crystal in a quality sufficient for the acoustic measurement,

there are no reliable experimental data for elastic constants of

the B19¢ martensite in the literature yet.

Given the lack of knowledge of elastic constants of the B19¢

martensite, theoreticians recently attempted to calculate them

from the first principles (Ref 5-7). All the available results seem

to suggest that martensite shall be the elastically harder phase,

which clearly contradicts the overwhelming experimental

evidence from tensile tests in the literature showing that

Youngs modulus of superelastic NiTi wire stretched beyond

This article is an invited paper selected from presentations at the International Conference on Shape Memory and Superelastic Technologies 2013, held May 20-24, 2013, in Prague, Czech Republic, and has been expanded from the original presentation.

Petr Sittner, Ludek Heller, and Jan Pilch, Institute of Physics, ASCR, Prague, Czech Republic. Caroline Curfs, ESRF, Grenoble, France; and Thiery Alonso and Denis Favier, Universite de Grenoble, Grenoble, France. Contact e-mail: [email protected]

1

the transformation plateau into stress-induced martensite

(Fig. 1a) is lower than in the austenite phase prior the plateau.

The low martensite modulus of NiTi has been a longstanding

puzzle in the SMA field. Hence, we decided to look at it more

closely in this work.

Wayne Metals, NiTi #1, straight annealed, d = 0.1 mm, was

used in present experiments. Youngs moduli of the austenite

and stress-induced martensite in these wires were evaluated by

three experimental methods (tensile tests, in situ synchrotron

x-ray diffraction, and dynamic mechanical analysis). Figure 1a

shows superelastic stress-strain curve of this wire stretched in

tension till fracture, yielding values of the static Youngs moduli

EA = 66.8 GPa (austenite) and EM = 24.8 GPa (martensite).

Electrical resistivity of the wire measured during the tensile test

is superimposed. Note that the electrical resistivity increases

with increasing stress both prior and after the plateau. It should

stay constant, if there was elastic deformation only. It is known

(Ref 8, 9) that, prior the plateau, this is due to the deformation

processes related with R-phase and due to twinning and

transformation after the plateau. So, it is obvious that evaluation

of the Youngs moduli from macroscopic responses in tensile

tests on NiTi wires is thus highly questionable.

An alternative way which can be used for evaluating the

elastic responses of solids regardless of the activity of other

deformation processes in the studied sample is the in situ x-ray

(neutron) diffraction method (Ref 10). In these methods, lattice

strain ehkl is evaluated (Eq. 1) from the relative changes of the

lattice spacing dhkl (position of the hkl diffraction peak in the

diffraction pattern) with increasing applied stress r. d0,hkl is the

lattice spacing in stress-free state.

ehkl ¼ dhkl d0;hklÞ=d0;hkl

ðEq 1Þ

To evaluate the strain component along thewire (load) axis, the

diffracting lattice planes must be oriented perpendicularly to the

load axis. Obviously, the strains ehkl evaluated from the changes of

lattice spacings (shift of diffraction peaks) are elastic strains only.

Since the intensity of the diffraction peak originates from a set of

equally oriented grains of a particular phase within the gage

volume of the polycrystalline wire, the lattice strains are oriented

and phase-sensitive values that are averaged over the gage volume.

If the values of lattice strains for various reflections are plot against

the applied stress r, the slopes of these dependences (Eq. 2) yield

so-called diffraction elastic moduli,Dhkl, characterizing the elastic

properties of thematerial. If thematerial is not toomuch elastically

anisotropic, then the slopes Dhkl for individual reflections are

similar each other and their average value approaches the Youngs

modulus of the polycrystal.

Dhkl ¼ r=ehkl ðEq 2Þ The in situ synchrotron x-ray experiments in this work were

performed using miniature deformation rig (Ref 11) installed on

high-resolution powder diffractometer ID31 at ESRF Grenoble.

The results for austenite and stress-induced martensite existing in

the thin NiTi wire under applied tensile stress are given in Fig. 2

and 1, respectively. The average value of austenite diffraction

moduli DA = 70 GPa is not that far from the value of Youngs

modulusmeasured in the stress-strain test. The stress-strain curves

in Fig. 2a and 1a are different, since theNiTi wirewas additionally

annealed (Fig. 2a) to avoid the R-phase (18 ms/125 W treatment

in Ref 11) complicating the analysis of the diffraction measure-

ments prior the stress plateau. Applying the same method to the

evaluation of elastic response of martensite is, however, a bit more

complicated, since it is not straightforward to measure the stress-

free lattice spacings d0,hkl (martensite does not exist without stress

at room temperature). On the other hand, we can measure more

lattice strain-stress dependences (Fig. 3), since there is more

martensite peaks in the martensite diffraction patterns (Fig. 1b).

d0,hkl for each martensite reflection was found by extrapolating the

linear lattice strain-stress dependences to zero stress. The results

clearly show that the orientation-dependent diffraction elastic

moduliDhkl of themartensite are systematically higher (DM 120

GPa), and the martensite phase is more elastically anisotropic than

the austenite. The results thus contradict the low value of the

martensite modulus evaluated from the tensile test.

Third method used to evaluate elastic properties of the NiTi

wire was dynamic mechanical analysis. Theoretically, the

dynamic modulus E¢ evaluated by this method from small

amplitude vibrations superimposed over the macroscopic static

stress-strain should not be affected by the activity of other

deformation mechanism acting in the wire. Although this is the

case for plasticity, it is not true for deformation processes derived

from the martensitic transformation which are accompanied by

Fig. 1 a) Tensile r-e curve of superelastic NiTi wire (FWM #1,

d = 0.1 mm) at room temperature. Electrical resistivity of the wire

measured during the tensile test is superimposed. (b) In situ x-ray

diffraction patterns evaluated under applied tensile stress (denoted by

points on r-e curve in (a) in axial geometry (diffracting planes per-

pendicular to wire axis)

2

the phase change or lattice orientation changes giving rise to the

mobile internal interfaces. Figure 4 shows the evolution of E¢

during a superelastic test on NiTi wire at room temperature till

fracture (Fig. 4a) and during cyclic superelastic test at T = 37 C

(Fig. 4b). Note that, prior the start of martensitic transformation,

the dynamic elastic modulus E¢ increases with stress at lower

temperature T = 19 C, while at higher temperature T = 37 C, it

decreases. This is the effect of the R-phase. The change of the E¢

with the applied stress during stress-induced B2-R transformation

has a form of U-shape. We see only the second branch of the U at

lower temperature T = 19 C (Fig. 4a), while only the first branch

of it at T = 37 C (Fig. 4b). If there is no R-phase, E¢ stays

constant during the elastic loading of the austenite (Fig. 2a). This

method can be used in principle to evaluate the elastic properties

(E¢) of the NiTi wire also in case of phase mixtures (1-7% strain)

within the transformation range, see the hysteretic variation ofE¢ in

Fig. 4b. The variation of E¢ with strain is not U-shaped but linear

due to thepropagationof localizeddeformation in shear bands.The

most important information to be inferred from Fig. 4, however, is

that, although the dynamic elastic modulus E¢ of martensite

increases with increasing stress beyond the plateau, it never

exceeds a maximum value of E¢ 50 GPa (Fig. 4a). The E¢

increases upon stressing the wire beyond the transformation

plateau since the twinning and transformation processes continue

beyond the plateau but their activity gradually expires. The

maximum of the E¢ 50 GPa observed at 10% strain corresponds

to their complete expiration not due to the onset of the plasticity.

3. Theoretical Calculations

mental results presented above, we tried to estimate Youngs

moduli of the B2 austenite phase and stress-induced monoclinic

B19¢ martensite phase in NiTi wire by theoretical calculations.

The idea is rather simple. First, we calculated single crystal

Fig. 2 Elasticity of the austenite evaluated from x-ray diffraction experiment on the high-resolution diffractometer ID31 at ESRF Grenoble, (a) tensile

r-e curve of the same NiTi wire additionally heat treated to avoid R-phase, Electrical resistivity of the wire measured during the tensile test is superim-

posed, (b, c) peak shifts measured in the diffraction experiment at tensile stresses denoted on the r-e curve in (a). Broad yellow profiles were obtained

after unloading after full superelastic cycle, (d) lattice strain-stress diagram showing linear ‘‘lattice plane responses’’ of various austenite hkl reflections

(Color figure online)

Fig. 3 Elasticity of martensite evaluated from the x-ray diffraction

experiment on the high-resolution diffractometer ID31 at ESRF Gre-

noble. Diffraction elastic moduli Dhkl of austenite and martensite

appearing as slopes of the lattice strain-stress dependence (measure-

ment points in Fig. 1a beyond the plateu)

3

Youngs modulus Ehkl along a given austenite crystal direction

hklA, and check how it changeswith the stress-inducedmartensitic

transformation in tension/compression. Ideally, this would corre-

spond to the slope of elastic response of austenite single crystal

loaded in tension/compression along the hkl direction prior and

after the stress-induced transformation. The single-crystal moduli

were calculated based on the knowledge of (i) crystal lattice

parameters and (ii) elastic constants of both austenite and

martensite phases, (iii) lattice correspondence between austenite

and martensite yielding information on how particular austenite

crystal direction transforms into the product phase, and (iv)

martensite variant selection rule telling which martensite variant

will form by the application of uniaxial tensile and compressive

strain along particular austenite crystal direction. Figures 7 and 8

inform the orientation and sense of loading dependence of the

single-crystal moduli. Finally, the polycrystalline Youngs moduli

are estimated taking into account grain constraints and textures.

3.1 Input Parameters

B19¢ martensite phases are listed in Table 1 including matrices

used for transforming Miller indexes hkl into vectors in

Cartesian system (xyz) aligned with lattice unit cells of

austenite and martensite. Matrix operators, lattice correspon-

dence, and related matrix operators are given in Table 2, and

finally, elastic constants of the austenite and martensite phases

taken from literature (Ref 5, 12, 13) are given in Table 3.

3.2 Martensite Variant Selection Rule

In order to evaluate how Youngs modulus of the austenite

single crystal will change with stress-induced martensitic

transformation when loaded along a specific direction in

tension/compression, one has to decide which one of the 12

martensite variants will form, i.e., one needs to adopt a

martensite variant selection rule. This is already an approxi-

mation, since we implicitly assume here that the austenite

single crystal will transform into a single martensite variant,

which yields maximum transformation strain into the load axis

direction and sense of loading (tension or compression).

In order to apply the above martensite variant selection rule,

we calculated orientation dependence of transformation strains

for all 12 martensite variants using transformation matrix

T xyz B2!B190 relating crystal directions of B2 austenite (uvw)T and

B19¢ martensite (UVW)T in the Cartesian system aligned with

B2 austenite unit cell (Eq. 3). In these calculations, lattice

parameters with related operators (Table 1) and austenite/

martensite lattice correspondence with related operators

(Table 2) are used.

u

v

w

0

hkl!xyz TB2 hkl!xyz Thkl

matrix Ui that is computed through polar decomposition of the

transformation matrix T xyz B2!B190 defined for each variant. Then,

engineering strain was used to calculate transformation strain

tensor ei i.e., ei = 1/2(Ui T + Ui) I, where I stands for 39 3

identity matrix. Orientation dependence of tensile/compressive

transformation strains was evaluated through projection of the

transformation strain tensor to all orientations i.e., tensile/

compressive transformation strain for variant i along direction

e = eTei e. The results for martensite variant 3 are shown in

Fig. 5. Orientation dependence of the maximum transformation

strain in compression (a) and tension (b) in a single quadrant of

austenite coordinate system are shown in Fig. 6. Note that (i)

transformations strains are statistically larger in tension than in

compression, and (ii) while one martensite variant is sufficient

to be considered within the basic stereographic triangle in

tension, three martensitic variants need to be considered in

compression.

From the above calculation, we know the load axis orienta-

tions within the martensite phase which corresponds to each

austenite crystal direction and sense of loading. Based on this, we

calculate orientation dependence of the single crystal Youngs

moduli using the elastic constants and show it in Table 3

(constants from Ref 5 were used). The results for martensite

variant 3 yielding largest strains in tension are shown in Fig. 7,

and for three martensite variants 1, 5, and 9 yielding larger

transformation strains in compression in are shown in Fig. 8.

Since plot of four surfaces in a single figure are difficult to inspect,

sections along {011} austenitic planes are shown.

Fig. 4 Tensile r-e curves of superelastic NiTi wire (NiTi #1, d = 0,

1 mm) with superimposed dynamic modulus E’ evaluated in DMA

experiment using frequency f = 30 Hz (a) at room temperature T = 19 C

till fracture and (b) cyclic test at ambient temperature T = 37 C

4

3.4 Effect of Grain Interactions and Texture on Polycrystalline Youngs Moduli

The next step should be to calculate Youngs modulus of

polycrystalline wire. Since the wire is not a set of isolated

crystals but a polycrystalline aggregate, in which the individual

single crystal grains mutually interact when exposed to external

loading, an averaging homogenization scheme must be adopted

to calculate homogenized polycrystalline Youngs modulus

(Ref 14-16). Although this topic has been widely addressed in

the literature, there are issues making it difficult to be applied to

NiTi wires as follows: (i) the crystal orientations are not

distributed randomly in the aggregate but some grain orienta-

tions prevail due to the strong texture of the thin wire (Fig. 9),

(ii) it is not realistic that whole grain transforms into one of the

12 lattice correspondent variants in Table 2, and (iii) it is not

realistic that the wire transforms fully to the martensite state

under stress. Typical NiTi wire texture results in a preferential

orientation of polycrystal grains along the 111A direction as

Fig. 9 shows. Although the latest averaging schemes published

in the literature go much far beyond the Voigt and Reuss

approximations allowing for taking into account the effects of

texture (Ref 16), grain size distribution (Ref 15), and even

multiphase microstructure (Ref 14) of the polycrystal, their

application to NiTi polycrystal in martensite state is still

problematic. There is one major critical issue-if we want to

compare the theoretical and experimental results, we need to

assure that the phase and twin interfaces do not move under the

increasing applied stress. Since we are lacking reliable inputs

for i-iii needed for homogenization and since the aim of this

work was mainly to clarify the long-lasting puzzle of the low

martensitic modulus of NiTi in material property tables,

polycrystalline Youngs moduli were not calculated but only

estimated in this work.

4.1 Youngs Modulus of the Wire in Austenite Phase

The values of the Youngs modulus of the polycrystalline

austenite phase evaluated by all methods converge around

E = 70 GPa. Theoretically calculated value of the

homogenized polycrystal Youngs modulus…